Predictive algorithms for determination of reflectance data from quantity of pigments within experimental dental resin composites
- Razvan Ghinea†1, 4Email author,
- Oscar Pecho†1,
- Luis Javier Herrera†2,
- Ana Maria Ionescu†1,
- Juan de la Cruz Cardona†1,
- María Purificación Sanchez†3,
- Rade D Paravina†4 and
- María del Mar Perez†1, 4
© Ghinea et al. 2015
Published: 13 August 2015
Being able to estimate (predict) the final spectrum of reflectance of a biomaterial, especially when the final color and appearance are fundamental for their clinical success (as is the case of dental resin composites), could be a very useful tool for the industrial development of these type of materials. The main objective of this study was the development of predictive models which enable the determination of the reflectance spectrum of experimental dental resin composites based on type and quantity of pigments used in their chemical formulation.
49 types of experimental dental resin composites were formulated as a mixture of organic matrix, inorganic filler, photo activator and other components in minor quantities (accelerator, inhibitor, fluorescent agent and 4 types of pigments). Spectral reflectance of all samples were measured, before and after artificial chromatic aging, using a spectroradiometer. A Multiple Nonlinear Regression Model (MNLR) was used to predict the values of the Reflectance Factors values in the visible range (380 nm-780 nm), before and after aging, from % Pigment (%P1, %P2, %P3 and %P4) within the formulation.
The average value of the prediction error of the model was 3.46% (SD: 1.82) across all wavelengths for samples before aging and 3.54% (SD: 1.17) for samples after aging. The differences found between the predicted and measured values of the chromatic coordinates are smaller than the acceptability threshold and, in some cases, are even below the perceptibility threshold.
Within the framework of this pilot study, the nonlinear predictive models developed allow the prediction, with a high degree of accuracy, of the reflectance spectrum of the experimental dental resin composites.
It has been reported that the composite restorative materials are one of the many successes of modern biomaterials research due to their capability to replace biological tissue in both appearance and function. In a recent review of treatment considerations for esthetic restorations it has been pointed out that at least half of the posterior direct restoration placement now rely on composite materials. Currently, methacrylate resin formulations dominate both the commercial market and research studies. The resin phase is composed primarily of dimethacrylate monomers (typically selected from Bis-GMA, BisEMA, and/or UDMA or a mixture of them) usually mixed with a low-viscosity reactive diluents (most commonly TEGDMA). These base monomers result in restorative materials with excellent mechanical properties, rapid polymerization, and low shrinkage.
Several authors implemented the use of experimental dental composites, as a continuous effort to understand the interrelationships among composition, resin viscosity, degree of conversion, shrinkage, flexural strength, fracture toughness, water sorption and solubility, etc. This type of materials were used to study the physical and mechanical properties of a new methacrylate monomer through comparisons with a commonly used Bis-GMA monomer, the effects of ceramic and porous fillers on the mechanical properties, the influence of irradiant energy on the degree of conversion, polymerization rate and shrinkage stress, the effect of co-initiator ratio on the polymer properties or the curing efficiency of dental resin composites. Furthermore, the use of a fluorescent agent was incorporated in the chemical formulation to study the influence of the fluorescent whitening agent on the fluorescent emission of resin composites.
Color prediction in dentistry is a research area that has barely been explored. So far it has been proven that the polymerization dependent color changes in resin composites can be successfully predicted using multivariable linear models of statistical inference. Also, in a recent study, the color change after tooth bleaching was predicted using a novel fuzzy logic model while other authors were able to predict the final color of 25 opaque feldspathic dental ceramic specimens fabricated by mixing six different pure shades in different concentrations.
The reflectance spectra is a physical characteristic of a sample, which provides valuable information with respect to the interaction of light (incident radiation) with the sample. Furthermore, based on the values of the reflectance factors for each wavelength of the visible spectrum, the final color of the sample under any available illuminant can be calculated. Therefore, being able to estimate (predict) the spectrum of reflectance of a biomaterial, especially in the case of materials whose color and appearance are fundamental for its clinical success (as it is the case of dental resin composite), could be a very useful tool for the industrial development of these type of materials. However, to the best of our knowledge, there is no available study on reflectance predictions for experimental dental resin composites.
Therefore, the main objective of this study is the development of predictive models which enable the determination of the reflectance spectrum in the visible range of experimental dental resin composites using as input data the type and quantity of pigments used in their chemical formulation.
Experimental dental resin formulation
Chemical components and their relative percentages by weight (% w/t) within the total mixture used to formulate the resin composites from this study.
Bisphenol A glycerolatedimethacrylate
Triethylene glycol dimethacrylate
SiO2 Glass Spheres [Φ: 9-13µm]
Pigment 1 (P1)
Pigment 2 (P2)
Pigment 3 (P3)
Pigment 4 (P4)
A total of 49 different mixtures of pigments were formulated by varying the relative amount of each of the four pigments. All chemical components were weighted using a high precision digital scale (BL60S, Sartorius AG, Goettingen, Germany) and carefully hand-mixed until a homogeneous mixture was obtained. All specimens were cylinder shaped with a diameter of 20 mm and 1.5 mm thickness. Each of the 147 specimens was packed in a custom built silicon mold in a glass plate sandwich with a mylar strip on both sides. The specimens were light cured at 1100 mW/cm2 for 60 seconds on each side using a LED light-curing unit (BluePhase, Ivoclar Vivadent AG, Schaan, Liechtenstein). In order to mimic a clinical situation and before storage, all samples were polished using a one-step diamond micro-polishing system (PoGo, Dentsply, USA), by applying light intermittent pressure at moderate speed during 40s.
All samples underwent an artificial chromatic aging. Specimens were placed inside an artificial aging chamber (Suntest XXL, ATLAS, USA) and subjected to artificial chromatic aging. The artificial aging cycle was defined as a 102 minutes dry and 18 minutes of water spray both under an artificial daylight simulator equivalent to CIE D65 Illuminant at 38 ± 3°C constant temperature and 50 ± 10% relative humidity, as described by ISO 4892-2 A1 and ISO 7491 Standards[12, 13].
The reflectance spectrum in the 380 nm-780 nm range of all specimens was measured inside a completely dark room using a spectroradiometer (PR 670, PhotoResearch, USA) and a spectrally calibrated reflectance standard (SRS-3, PhotoResearch, USA). Specimens were placed on a custom built sample holder, 40 cm away from the spectroradiometer and illuminated using a Xe-Arc Light Source (Oriel Research, Newport Corporation, USA). The illuminating/measuring geometry corresponded to CIE 45°/0°. The aperture of the spectroradiometer was set to 1°, which allowed the measurement of a central spot (measuring field) of the specimen of approximately 0.7 cm.
Short-term repeated reflectance measurements without replacement were performed and each sample was measured three times. As three samples of each group were produced, this gave a total of 9 recording for each type and the results were averaged. This procedure was performed before and after the chromatic artificial aging procedure.
Color and color difference calculations
Color calculations (chromatic coordinates CIE L*, a* and b*) for both real and predicted reflectance spectra were performed in base of the CIE D65 Standard Illuminant and the CIE Colorimetric 2° Standard Observer assumptions.
where ΔL', ΔC' and ΔH' are the differences between the two samples forming the pair in lightness, chroma and hue, and R T is the rotation function which accounts for the interaction between chroma and hue differences in the blue region. The weighting functions S L , S C and S H adjust the total color difference for variation in the location of the color difference pair in L', a'and b' coordinates and the parametric factors K L , K C and K H are correction terms for experimental conditions. For calculations made in this study, all the parametric factors were set to 1. All the discontinuities due to mean hue computation and hue-difference computation pointed out and characterized by Sharma and collaborators were taken into account when the calculations with the CIEDE2000 color difference formula were performed.
Design of the predictive models
Samples were divided into a Training (Active) Group, which contained 44 samples (sample 1 to 44) from the total of 49 samples available, and a Testing (Validation) Group, which contained 5 samples from the total of 49 samples available (Sample 45 to 49). Samples in the Testing Group present a combination of the 4 pigments. In all cases, the Active (Training) Group was used to build the predictive model while the Validation Group was used exclusively for testing the appropriate functioning of the model as well as its accuracy.
A Multiple Nonlinear Regression Model (MNLR) was used to predict the values of the Reflectance Factors values in the visible range (380 nm-780 nm) before and after aging from % Pigment (%P1, %P2, %P3 and %P4) within the formulation.
Y is the predicted variable: Reflectance Factors values in the visible range (380 nm-780 nm) at 2 nm step the before and after aging;
Xi are the input variables: %P1, %P2, %P3 and %P4;
pr1 ... pr17 are the parameters of the model.
The models were built using the Training Group and tested using the Validation Group. The model was considered to be accurate after 200 iterations were performed and/or a convergence of 0.00001 was achieved.
A total of 402 models (one for each Reflectance Factor before and after aging) were designed. All the Multiple Nonlinear Regression predictive models were designed using a commercial software (XLSTAT, Addinsoft, USA).
Results and discussion
In dentistry, it would be ideal to achieve a restoration that has identical colors as the tooth structure under various illumination conditions, within at least acceptable limits, but more preferably within limits of perceived color difference. Although the importance of the pigments on the final color and appearance of the dental resin composite is well known, there is no research study available which made use of coloring pigments when formulating the experimental dental resin composites. Therefore, in this study, the use of pigments was included in the chemical formulation of the resin composites.
The research in science and biomedical applications often involves using controllable and/or easy to measure variables (input factors) to explain, regulate or predict the behavior of other variables (output factors or dependent variables). When dealing with a reduced number of input factors which are not significantly redundant and have a strong relationship with the output variables, the MNLR is one of the best options to take into account for modeling the data.
The correlation between variables, when biomaterials are studied, is considered to be strongly direct if the value of the Pearson Coefficient exceeds 0.7 and is considered to be strongly inverse if the value of the Pearson Coefficient is lower than -0.7. As it can be observed in Figure 1, for the 5 samples included in the testing group (Validation Group) before aging, there is a strong inverse correlation between the quantity of the fourth Pigment (%P4) and reflectance factors of wavelengths between 525 nm-650 nm. This implies that higher quantities of Pigment 4 within the mixture of the experimental resin composite will decrease the values of the reflectance factors between the specified interval, affecting the lightness value of the sample and generating an orange-reddish color shift. Also, a strong correlation usually is associated with increased performance of the predictive model, but no conclusion should be drawn before analyzing the other parameters of the quality of fit, such as goodness of fit or relative residuals.
Our visual system is also subject to many visual complications that can produce systematic distortions in the visual estimates of the quality of a fit. However, as it can be observed in Figures 3, 4, 5, 6, 7, the quality of the fit is excellent for almost the entire spectrum, providing accurate estimates of the Reflectance Factors for all wavelengths.
Several MNLR predictive models have been developed, which accurately predicted the reflectance spectrum of the manufactured experimental dental resin composites. These models are very helpful when, in a laboratory situation, the chromatic behavior of the samples needs to be controlled. In this study, we considered the pigments as the main responsible (not exclusive) of the final color of the composites, and therefore we centered the study on the influence of the four types of pigments on the final color of the experimental dental resin composites.
In a study on the perceptibility and acceptability of tooth color differences using computer-generated pairs of teeth with simulated gingival displayed on a calibrated monitor, Lindsey and Wee established that ΔL* = 1.0, Δa* = 1.0 and Δb* = 2.6 units are considered as 50:50% perceptibility threshold for the human eye. In our study, the differences between the predicted and the measured values of the chromatic coordinates exceeded the lightness threshold for 40% of the studied samples (both before and after aging). For the b* chromatic coordinate, 80% of the samples presented differences which were unable to be perceived by a human observer with normal color vision, while for the red-green axis (a* coordinate) all the studied samples exhibited differences bellow the perceptibility threshold for this coordinate, independently if the sample were analyzed before or after the aging procedure was applied.
The visual 50:50% acceptability thresholds for lightness, chroma and hue in dentistry were established as ΔL' = 2.92, ΔC' = 2.52 and ΔH' = 1.90 units. The differences found between the predicted and the measured values are smaller than the acceptability thresholds for lightness and hue, independently if the samples are analyzed before or after the aging procedure was applied. In the case of chroma differences, for one of the samples included in the Validation Group, the computed difference exceeded the acceptability threshold, while all the other four samples exhibited values considerably lower than the threshold.
It has to be mentioned that the range of application of the proposed predictive models is limited, since they are designed to work exclusively with the experimental dental resins developed in this study. It is necessary to expand the present work with further studies on multiple areas, such as varying the materials used for the formulation, varying amounts of both the organic matrix and the inorganic filler as well as the quantities of the other components used in the chemical formulation.
It would also be interesting to study more carefully the behavior of the different pigments, through a wider range of combinations between them and, on the other hand, other pigments can be used for colorimetric formulations. Another development path for future studies is an improved experimental design, in terms of better coverage of the dental color space with the manufactured samples. A proper distribution of the samples within the area of interest of the color space will allow the use of newer, more accurate and reliable predictive methods, such as Fuzzy Logic.
However, one should not underestimate the importance of the exact knowledge of the reflectance spectrum of the samples to be analyzed, since by knowing the reflectance factor values for any wavelength within the visible spectrum (380 n-780 nm) we are able to calculate the values of the chromaticity coordinates under any illuminant (not only the daylight simulator - CIE D65) and for any CIE Colorimetric Standard Observer. These calculations have the potential to provide important additional information, depending on the objective of the study. In this sense, if the study is intended to cover a widely range of colorimetric coordinates under different Standard Illuminants and with different Standard Observers, it is advisable to design predictive models for reflectance factors at each wavelength, which will allow to make various calculations based on the equations provided by the International Commission on Illumination (CIE).
Soft science applications involve so many variables that it is not practical to seek a model which explicitly relates them all. The Multiple Nonlinear Regression is one of the possible solutions and although it is continuously evolving as a statistical modeling technique, there are other fields which can provide also good results, such as principal components regression, maximum redundancy analysis, methods which handle the colinearity in regression, such as the ridge regression, or newer methods, such as the neural networks. The neural networks are probably the strongest competitors for MNLR in terms of flexibility and robustness of the predictive models, but they do not explicitly incorporate a linear extraction of latent factors - that is dimension reduction.
Within the framework of this preliminary study, the nonlinear predictive models developed allow the prediction, with a high degree of accuracy, of the reflectance spectrum of the experimental dental resin composites (average error <3.54% across all wavelengths of the visible spectrum). The differences found between the predicted and measured values of the chromatic coordinates are smaller than the acceptability threshold established for this type of materials and, in some cases, are even below the perceptibility threshold. These results open the way for custom design of dental resin composites, with multiple direct and immediate clinical applications, such as the manufacture of dental shade guides, development of new dental materials, and finally, performing dental restorations that perfectly match the color of their surrounding dental structures. However, before bringing these materials to the clinic, the present study has to be complemented with studies on other physical and chemical properties of the material, such as polymerization shrinkage, hardness, wear resistance, degree of polymerization, temporal and thermo chromatic stability, etc.
The research presented in this study was partially funded by CEI BioTic 94, JA-TEP 1136, PYR-2014-12 and MAT2013-43946-R research grants.
Publication of this article was supported by Spanish Ministry of Economy and Competitiveness MAT2013-43946-R Grant.
This article has been published as part of BioMedical Engineering OnLine Volume 14 Supplement 2, 2015: Select articles from the 2nd International Work-Conference on Bioinformatics and Biomedical Engineering (IWBBIO 2014). The full contents of the supplement are available online at http://www.biomedical-engineering-online.com/supplements/14/S2.
- Cramer NB, Stansbury JW, Bowman CN: Recent advances and developments in composite dental restorative materials. Journal of Dental Research. 2011, 90 (4): 402-416. 10.1177/0022034510381263.View ArticleGoogle Scholar
- Sadowsky SJ: An overview of treatment considerations for esthetic restorations: a review of the literature. Journal of Prosthetic Dentistry. 2006, 96 (6): 433-442. 10.1016/j.prosdent.2006.09.018.View ArticleGoogle Scholar
- Atai M, Nekoomanesh M, Hashemi SA, Amani S: Physical and mechanical properties of an experimental dental composite based on a new monomer. Dental Materials. 2004, 20 (7): 663-668. 10.1016/j.dental.2003.08.008.View ArticleGoogle Scholar
- Zandinejad AA, Atai M, Pahlevan A: The effect of ceramic and porous fillers on the mechanical properties of experimental dental composites. Dental Materials. 2006, 22 (4): 382-387. 10.1016/j.dental.2005.04.027.View ArticleGoogle Scholar
- Calheiros FC, Daronch M, Rueggeberg FA, Braga RR: Influence of irradiant energy on degree of conversion, polymerization rate and shrinkage stress in an experimental resin composite system. Dental Materials. 2008, 24 (9): 1164-1168. 10.1016/j.dental.2008.01.006.View ArticleGoogle Scholar
- Schneider LF, Cavalcante LM, Consani S, Ferracane JL: Effect of co-initiator ratio on the polymer properties of experimental resin composites formulated with camphorquinone and phenyl-propanedione. Dental Materials. 2009, 25 (3): 369-375. 10.1016/j.dental.2008.08.003.View ArticleGoogle Scholar
- Schneider LF, Cavalcante LM, Prahl SA, Pfeifer CS, Ferracane JL: Curing efficiency of dental resin composites formulated with camphorquinone or trimethylbenzoyl-diphenyl-phosphine oxide. Dental Materials. 2012, 28 (4): 392-397. 10.1016/j.dental.2011.11.014.View ArticleGoogle Scholar
- Park MY, Lee YK, Lim BS: Influence of fluorescent whitening agent on the fluorescent emission of resin composites. Dental Materials. 2007, 23 (6): 731-735. 10.1016/j.dental.2006.06.028.View ArticleGoogle Scholar
- Ghinea R, Ugarte L, Ionescu AM, Cardona JC, Perez MM: Development of a linear model to predict polymerization dependent color changes. Proceedings of SCAD. 2010, Newport Beach, USAGoogle Scholar
- Herrera LJ, Pulgar R, Santana J, Cardona JC, Guillen A, Rojas I, Perez MM: Prediction of color change after tooth bleaching using fuzzy logic for Vita Classical shades identification. Applied Optics. 2010, 49 (3): 422-429. 10.1364/AO.49.000422.View ArticleGoogle Scholar
- Wee AG, Chen WY, Johnston WM: Color formulation and reproduction of opaque dental ceramic. Dental Materials. 2005, 21 (7): 665-670. 10.1016/j.dental.2004.09.003.View ArticleGoogle Scholar
- ISO 4892-2:2013. Plastics - Methods of exposure to laboratory light sources - Part 2. Xenon-arc lamps. 2013, International Organization for StandardizationGoogle Scholar
- ISO 7491:2000. Dental materials -- Determination of colour stability. 2000, International Organization for StandardizationGoogle Scholar
- CIE - International Comission on Illumination: Technical Report: Colorimetry. 2004, Vienna, AustriaGoogle Scholar
- Sharma G, Wu W, Dalal E: The CIEDE2000 color-difference formula: Implementation notes, supplementary test data, and mathematical observations. Color Research and Application. 2004, 30 (1): 21-30.View ArticleGoogle Scholar
- Johnston WM: Color measurement in dentistry. Journal of Dentistry. 2009, 37 (SUPPL. 1): e2-e6.View ArticleGoogle Scholar
- Schunn C, Wallach D: Evaluating goodness-of fit in comparison of models to data. 2005, Psychologie der Kognition: Reden and Vorträge anlässlich der Emeritierung von Werner Tack, University of Saarland Press, Saarbrücken, GermanyGoogle Scholar
- Lindsey DT, Wee AG: Perceptibility and acceptability of CIELAB color differences in computer-simulated teeth. Journal of Dentistry. 2007, 35 (7): 593-599. 10.1016/j.jdent.2007.03.006.View ArticleGoogle Scholar
- Ghinea R, Perez MM, Herrera LJ, Rivas MJ, Yebra A, Paravina RD: Color difference thresholds in dental ceramics. Journal of Dentistry. 2010, 38 (SUPPL. 2): e57-e64.View ArticleGoogle Scholar
- Perez MM, Ghinea R, Herrera LJ, Ionescu AM, Pomares H, Pulgar R, Paravina RD: Dental ceramics: A CIEDE2000 acceptability thresholds for lightness, chroma and hue differences. Journal of Dentistry. 2011, 39 (SUPPL. 3): e37-e44.View ArticleGoogle Scholar
- Hoerl AE, Kennard RW: Ridge Regression - Biased Estimation for Nonorthogonal Problems. Technometrics. 2000, b42 (1): 80-86.View ArticleMathSciNetMATHGoogle Scholar
- Haykin S: Neural networks: A comprehensive foundation. 1994, New York: MacMillanGoogle Scholar
- Frank IE, Friedman JH: A Statistical View of Some Chemometrics Regression Tools. Technometrics. 1993, 35 (2): 109-135. 10.1080/00401706.1993.10485033.MATHView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.